DOI: 10.17188/1475860
title: Materials Data on SrCa3Mn4O10 by Materials Project

description: SrCa3Mn4O10 crystallizes in the triclinic P1 space group. The structure is three-dimensional. there are eight inequivalent Sr2+ sites. In the first Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.45–3.17 Å. In the second Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.45–3.15 Å. In the third Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.40–2.90 Å. In the fourth Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.41–3.11 Å. In the fifth Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.46–3.05 Å. In the sixth Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.45–3.16 Å. In the seventh Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.44–3.16 Å. In the eighth Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.44–3.16 Å. There are twenty-four inequivalent Ca2+ sites. In the first Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.36–2.90 Å. In the second Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.33–2.85 Å. In the third Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.35–2.91 Å. In the fourth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.31–2.91 Å. In the fifth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.35–2.89 Å. In the sixth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.41–2.84 Å. In the seventh Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.36–2.89 Å. In the eighth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.37–2.88 Å. In the ninth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.31–2.93 Å. In the tenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.37–2.90 Å. In the eleventh Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.31–2.86 Å. In the twelfth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.36–2.91 Å. In the thirteenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.37–2.88 Å. In the fourteenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.36–2.89 Å. In the fifteenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.37–2.89 Å. In the sixteenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.35–2.90 Å. In the seventeenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.37–2.88 Å. In the eighteenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.38–2.83 Å. In the nineteenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.36–2.83 Å. In the twentieth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.37–2.88 Å. In the twenty-first Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.33–2.90 Å. In the twenty-second Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.33–2.86 Å. In the twenty-third Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.36–2.90 Å. In the twenty-fourth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.37–2.89 Å. There are thirty-two inequivalent Mn3+ sites. In the first Mn3+ site, Mn3+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with four MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 10–11°. There are a spread of Mn–O bond distances ranging from 1.96–2.05 Å. In the second Mn3+ site, Mn3+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with four MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 6–9°. There are a spread of Mn–O bond distances ranging from 1.96–2.12 Å. In the third Mn3+ site, Mn3+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with four MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 10–11°. There are a spread of Mn–O bond distances ranging from 1.97–2.09 Å. In the fourth Mn3+ site, Mn3+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with four MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 7–11°. There are a spread of Mn–O bond distances ranging from 1.96–2.10 Å. In the fifth Mn3+ site, Mn3+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with four MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 9–10°. There are a spread of Mn–O bond distances ranging from 1.96–2.08 Å. In the sixth Mn3+ site, Mn3+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with four MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 10–12°. There are a spread of Mn–O bond distances ranging from 1.96–2.07 Å. In the seventh Mn3+ site, Mn3+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with four MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 9–12°. There are a spread of Mn–O bond distances ranging from 1.97–2.06 Å. In the eighth Mn3+ site, Mn3+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with four MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 7–10°. There are a spread of Mn–O bond distances ranging from 1.95–2.10 Å. In the ninth Mn3+ site, Mn3+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with four MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 9–12°. There are a spread of Mn–O bond distances ranging from 1.97–2.08 Å. In the tenth Mn3+ site, Mn3+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with four MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 7–11°. There are a spread of Mn–O bond distances ranging from 1.97–2.12 Å. In the eleventh Mn3+ site, Mn3+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with four MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 9–10°. There are a spread of Mn–O bond distances ranging from 1.96–2.09 Å. In the twelfth Mn3+ site, Mn3+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with four MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 9–11°. There are a spread of Mn–O bond distances ranging from 1.96–2.09 Å. In the thirteenth Mn3+ site, Mn3+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with four MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 9–11°. There are a spread of Mn–O bond distances ranging from 1.96–2.08 Å. In the fourteenth Mn3+ site, Mn3+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with four MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 9–12°. There are a spread of Mn–O bond distances ranging from 1.97–2.12 Å. In the fifteenth Mn3+ site, Mn3+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with four MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 10–11°. There are a spread of Mn–O bond distances ranging from 1.96–2.05 Å. In the sixteenth Mn3+ site, Mn3+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with four MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 6–10°. There are a spread of Mn–O bond distances ranging from 1.95–2.10 Å. In the seventeenth Mn3+ site, Mn3+ is bonded to four O2- atoms to form MnO4 tetrahedra that share corners with two MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 29–31°. There are a spread of Mn–O bond distances ranging from 1.93–2.04 Å. In the eighteenth Mn3+ site, Mn3+ is bonded to four O2- atoms to form MnO4 tetrahedra that share corners with two MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 23–27°. There are a spread of Mn–O bond distances ranging from 1.90–2.00 Å. In the nineteenth Mn3+ site, Mn3+ is bonded to four O2- atoms to form MnO4 tetrahedra that share corners with two MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedral tilt angles are 30°. There are a spread of Mn–O bond distances ranging from 1.94–2.05 Å. In the twentieth Mn3+ site, Mn3+ is bonded to four O2- atoms to form MnO4 tetrahedra that share corners with two MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 23–28°. There are a spread of Mn–O bond distances ranging from 1.91–2.01 Å. In the twenty-first Mn3+ site, Mn3+ is bonded to four O2- atoms to form MnO4 tetrahedra that share corners with two MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 29–30°. There are a spread of Mn–O bond distances ranging from 1.92–2.04 Å. In the twenty-second Mn3+ site, Mn3+ is bonded to four O2- atoms to form MnO4 tetrahedra that share corners with two MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 25–30°. There are a spread of Mn–O bond distances ranging from 1.93–2.02 Å. In the twenty-third Mn3+ site, Mn3+ is bonded to four O2- atoms to form MnO4 tetrahedra that share corners with two MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 30–31°. There are a spread of Mn–O bond distances ranging from 1.92–2.04 Å. In the twenty-fourth Mn3+ site, Mn3+ is bonded to four O2- atoms t